Atti dell’Accademia Peloritana dei Pericolanti Classe di Scienze Fisiche, Matematiche e Naturali Vol. LXXXVI, C1S0801008 (2008) - Suppl. 1

THERMODYNAMICS OF HETEROGENEOUS AND ANISOTROPIC NONLINEAR FERROELASTIC CRYSTALS

MAUROFRANCAVIGLIA^{[a]}ANDLILIANARESTUCCIA^{[b]}*

ABSTRACT. In a previous paper, in a geometrized framework for the description of sim- ple materials with internal variables, the specific example of ferroelastic crystals with anisotropy grain-tensors `a la Maruszewski was considered and the relevant structure of the entropy 1-form was derived. In this contribution the linear morphism defined on the fibre bundle of the process and the transformation induced by the process are obtained as new results within the geometrical model. Furthermore, Clausius-Duhem inequality for these media is exploited, and, using a Maugin technique (see also Colemann-Noll proce- dure), the laws of state, the extra entropy flux and the residual dissipation inequality are worked out. Finally, following Maugin, the heat equation in the first and the second form is derived.

1. Introduction

In a previous paper [1] a geometrization technique for thermodynamics of simple ma- terials with internal variables [2]-[8] was applied to the specific example of ferroelastic crystals (see [9]-[13]) and the expressions for the existence of an entropy function and the entropy 1-form were derived. The model of ferroelastic crystals developed in [9]-[13] is based on a concept of anisotropy grain structure first introduced in [14]. The idea used consists in the assumption that the body as a whole is homogeneous and isotropic, where there exist particular physical fields responsible for its internal structure and geometry, described by internal variables [14]. In this way the balance equations for the mass, the momentum, the moment of momentum and the internal energy, and the rate equation for the heat flux vector are supplemented by the evolution equations for the anisotropy-grain tensors forming altogether a coupled system of equations describing the behavior of the ferroelastic body considered. The proper form of these equations has been derived from the thermodynamical models presented in [9]-[13]. The stress wave propagation and some explicit examples of stress tensors in these models were considered in [13] and [10]-[12].

In this contribution the linear morphism defined on the fibre bundle of the process and the transformation induced by the process are obtained as new results within the geometrical model developed in [1] for the description of ferroelastic crystals (see also [15] and [16]

for the geometrization technique applied). Furthermore, we exploit the Clausius-Duhem inequality for these media and, using a Maugin technique [17] (see also Colemann-Noll procedure in [18]), we derive the extra entropy flux, the residual dissipation inequality and the laws of state, where as relevant result the contributions in the total stress tensor ex- pressed in terms of internal variables are rewritten in terms of macroscopic variables (the

1

Duhamel-Neumann tensor stress and the nonlinear strain tensor). Finally, the heat equation in the first and the second form is obtained following Maugin [17].

2. The anisotropy-grain tensor model

FIGURE1. Internal structure of the body. Anisotropic character of grains (after [19]) Now, we recall the model developed by Maruszewski in [14] for heterogeneous and/or anisotropic media. The ferroelastic crystal can be defined as a crystal which has at least two orientation states that differ from each other with respect to at least one of the compo- nents of the spontaneous strain tensor. A suitably oriented uniaxial stress can often switch one ferroelastic orientation state to another so that the ferroelastic domains can be made to grow or shrink by applying such a driving force in complete analogy with domains in fer- roelectric and ferromagnetic materials. In [14] it was assumed that a heterogeneous body B is formed by several kinds of grains with different anisotropies (see Fig.1 after [19]).

The families of different species of grains are labeled by an index α (α running from 1 to an integer r, the total number of species) and the families of different anisotropies occur- ring in the body are labeled by a further index β (β running from 1 to s, the total number of anisotropies). A third index γ is introduced to distinguish between line anisotropies (γ = 1) and planar anisotropies (γ = 2). Now, following Maruszewski, the body as a whole is regarded as homogeneous and isotropic in which particular physical fields re- sponsible for its internal structure and geometry exist. Such fields are modeled by so-called internal variables, having tensorial character and defined by the Anisotropy-Grain tensor (or shortly, the AG-tensor)

(1) Γ^{αβ}(t, x) = V^{α}n^{αβ}(t, x)A^{βγ}, (α = 1, 2, ..., r; β = 1, 2, ..., s; γ = 1, 2),
where there is no summation over α and β. In equation (1) V^{α}denotes the characteristic
dimension of the α-grain or domain field possessing β anisotropy (in the 3D case it is the
characteristic volume of the α-grain, in the 2D case the characteristic surface S^{α}of the
α-grain, in the 1D case the characteristic length L^{α}(diameter) of the α-grain). Finally,
n^{αβ}(t, x) is the number density of the α-grain with anisotropy β defined as follows
(2)

3D : n^{αβ}(t, x) = dN^{αβ}(t, x)

dV^{α} , 2D : n^{αβ}(t, x) = dN^{αβ}(t, x)

dS^{α} , 1D : n^{αβ}(t, x) = dN^{αβ}(t, x)
dL^{α} ,
where N^{αβ}(t, x) is the corresponding total number of grains with β anisotropies.

Moreover, in equation (1) the tensor A^{βγ} reflects the anisotropy (geometry) of a grain and it is
defined as follows (see Fig.2 ): A^{β1} = t^{β}⊗ n, A^{β2} = n^{β} ⊗ n, for line anisotropies and for
planar anisotropies, respectively, with n the unit normal vector to the the cross section δB of the
domain dB of the body, t^{β} the tangent unit vector to the line anisotropic structure β and n^{β} the

FIGURE 2. Element dB of a domain in the case of line (b) and planar (c) anisotropies. δB is the cross-section of dB (after [14])

FIGURE3. Line anisotropy model (after [13])

unit normal vector to the surface anisotropy. Γ^{αβ}may be regarded as a sort of order parameter for
ferroelasticity, in the sense of Landau [20], provided one assumes that anisotropies disappear in the
ferroelastic crystal when θ reaches the critical value θc( i.e., A^{βγ}= 0 for θ ≥ θc). A few specific
examples have been analyzed in detail in [9], [12] and in [13]. Let us consider now a case of line
anisotropy of the bodyspontaneously deformed (see Fig. 3 after [13]). We assume that all the lines
or the fibers (infinite quantity because of the continuous model) are placed in the plane x1x2 and
parallel to x3-axis. Since we consider a single-domain (one grain) medium, the anisotropy-grain
tensor reads

(3) Γ^{β}_{ij}= Γij= A^{β1}_{ij}(x, t) = t^{β}⊗ n, t^{β}= {0, 0, 1}, n = {0, 1, 0}.

Hence, only Γ326= 0 since

(4) A^{β1}=

0 0 0

0 0 0

0 1 0

.

Let us consider now a case of plane anisotropy of the body spontaneously deformed (see Fig. 4 after
[13]). We assume that all the planes (infinite quantity because of the continuous model) are parallel
to the plane x1x3. Since we consider a single grain medium, the anisotropy-grain tensor reads
(5) Γ^{β}_{ij}= Γij= A^{β2}_{ij}(x, t) = n^{β}⊗ n, n^{β} = {0, 1, 0}, n = {0, 1, 0}.

Hence, only Γ226= 0 since

(6) A^{β2}=

0 0 0

0 1 0

0 0 0

.

In the case of an anisotropic layered structure of a grain, the total anisotropy of a grain is described

FIGURE4. Plane anisotropy model (after [13])

FIGURE 5. Anisotropic layered structure (schematic draw): (1) grain, (2) pla- nar anisotropy, (3) line anisotropy (after [14])

by the superposition of the line and planar anisotropies (see [14]). Hence, we can introduce the total
anisotropy tensor as A^{β}_{ij}= A^{β1}_{ij} + A^{β2}_{ij}. A simple example is presented on Fig. 5 (see [14]), where

t^{β} = {0, 0, 1}, n = {0, 1, 0}, n^{β}= {0, 1, 0}, A^{β1}=

0 0 0

0 0 0

0 1 0

, A^{β2}=

0 0 0

0 1 0

0 0 0

. Hence, the total anisotropy tensor reads

(7) A^{β}_{ij}= A^{β1}_{ij} + A^{β2}_{ij} =

0 0 0

0 1 0

0 1 0

.

It shows that it is possible to describe quite complex structures. In the limiting case of homogeneous body, when the body does not consist of grains we have (3D) [14]

(8) V^{αβ} = V, n^{αβ}(t, x) =N^{αβ}(t, x)

V , N^{αβ}(t, x) = 1, Γ^{αβ}(t, x) = Γ^{β} = A^{βγ}.
It means that in such a case the tensor Γ^{αβ}describes, as internal variable, only the anisotropy.

In the other limiting case of the isotropic body the tensor A^{βγ}takes the following form:

A^{βγ}= I, hence Γ^{α}= V^{α}n^{αβ}I describing only the grain structure of the body.

The above defined anisotropy-grain tensor Γ^{αβ}can describe heterogeneous and anisotropic
media as an internal variable in many situations. Evolution of grain structure and anisotropy
of materials occurs during many processes accompanied by mechanical deformation and
thermal treatments. Such phenomena as: recrystallization, phase transitions, twinning,
grain growth and similar phenomena, are typical during annealing, cooling, cold-working
or plastic deformations [14]. The models of ferroelastic bodies may have relevance in the

study of concrete materials such as, e.g., steel, martensitic plates in metals and others. On Fig. 6 the evolution of structure and anisotropy in materials is shown (after [21]).

FIGURE6. Evolution of a microstructure of steel during cooling (after [21])

3. Fundamental laws

In [10], in the framework of the extended rational thermodynamics with internal vari- ables, using the standard Cartesian tensor notation in a rectangular coordinate system, a model was developed for a heterogeneous and anisotropic non linear thermoelastic body, in which the following fields interact with each other: the elastic field described in the case of finite deformations by the total stress tensor tij and the nonlinear Euler strain tensor Eij; the thermal field described by the temperature θ and the heat flux qi; the grain- anisotropy field described by the internal variable Γij, in the case that there exists one type (size) of grain ( α = 1) and one kind of anisotropy (β = 1). Thus, the independent variables are represented by the set

(9) C = {Eij, θ, θ,i, qi, Γij} .

The specific choice shows that the relaxation properties of the thermal field (second sound) are taken into account in agreement with the general philosophy of the extended thermo- dynamics. The corresponding effects for the mechanical field and for the anisotropy-grain field are ignored, i.e. viscous properties of the body are excluded from the considera- tion and the field Γij is not of kinetic character. All the processes occurring in the body considered are governed by two groups of laws. The first one deals with the balance laws:

the continuity equation

(10) µ + µv˙ i,i= 0,

where µ is the mass density and v = ˙u (being u = (ui) the displacement vector and the superimposed dot denotes the material derivative);

the momentum balance

(11) µ ˙v − divt − f = 0,

where f denotes the body force and t is the total stress tensor given by

(12) t = T − σ^{T E}− σ^{HA}

(see equation (2.19) of reference [10] for the law of state (12) defining the total stress tensor t ). First, we mention that the model developed in [10] refers to large deformations, so that T = kTijk is here the symmetric Duhamel-Neumann stress tensor defined as

(13) T_{ij}= µ ∂Ψ

∂Eij

.

The extra terms in (12) account for the grain-anisotropy. The term σ^{T E}corresponds to the
thermoelastic stressand in components kσ_{ij}^{T E}k is given by

(14) σ^{T E}_{ij} = Π^{q}_{s}qjEsi+ Π^{q}_{i}qkEjk,

where q = (qi) is the heat flux vector, Π^{q} = (Π^{q}_{i}) is the affinity defined by Π^{q}_{i} = µ^{∂Ψ}_{∂q}

i, and Ψ = e − θS , e and S are the Helmholtz free energy, the internal energy and the entropy per unit mass, respectively. In [10] it was derived that Ψ depends on the following set of variables Ψ = Ψ(E, θ, q, Γ). The non linear Eulerian strain tensor Eij

is a symmetric rank-2 tensor defined by Eij = ^{1}_{2}(ui,j+ uj,i− um,ium,j). It describes
the elastic fieldin the case of finite deformations. In the general case (α kinds of grains
and β anisotropies), the second extra term of (12) accounts for the interaction of the
grain-anisotropy field with the mechanical field. It is defined by

σ_{ij}^{HA}=X

α,β

σ_{ij}^{HAαβ} with σ^{HAαβ}_{ij} = η_{rs}^{αβ}Γ^{αβ}_{js}E_{ri}+ η_{rs}^{αβ}Γ^{αβ}_{rj}E_{si}+ η_{ri}^{αβ}Γ^{αβ}_{rs}E_{js}

and η_{ij}^{αβ}= µ ^{∂Ψ}

∂Γ^{αβ}_{ij} an affinity;

the moment of momentum balance ε_{ijk}t_{jk}= 0,

which results from the assumption that the medium has no spin, microrotational or other skew-symmetric features, it means that the total stress tensor is symmetric (see equations (3.3)-(3.6) in [10], where, using the laws of state, a constitutive relation was worked out for a symmetric total stress tensor according to particular assumptions);

the internal energy balance

(15) µ ˙e − p_{(i)}+ divq − µr = 0,

with r the heat radiation per unit of mass and p(i)the power of internal forces defined by
(16) p(i)= t · L = (T − σ^{T E}− σ^{HA}) · L,

where L = ∇v is the gradient of the velocity. In the following sections we use the relation
L = ˙FF^{−1} expressing L in terms of the gradient of the deformation F.

A second group of laws deals with the rate properties of the heat flux and the anisotropy- grain field

(17) q= Q(C),^{∗} Γ= G(C),^{∗}

where ^{∗}q_{i}= ˙q_{i}− Ω_{ij}q_{j}, Γ^{∗}ij= ˙Γ_{ij}− Ω_{ik}Γ_{kj}+ Γ_{ik}Ω_{kj}, Ω_{ij} = ^{1}_{2}(v_{i,j}− v_{j,i}) is the
antisymmetric part of L_{ij} = v_{i,j} and the superimposed asterisk indicates the Zaremba-
Jaumann time derivative (see [22]). To be sure that the physical processes occurring in the
body considered are real, all the admissible solutions of the proposed evolution equations
have to satisfy the following entropy inequality

(18) µ ˙S + ∇ · JS ≥ 0, where JS = 1 θq + k,

with JS the entropy flux and k an additional term called extra entropy flux density (see [17] and [23]-[26]). The set of the constitutive functions are

(19) Z = {t, e, S, k, Q, G} .

In [9]-[13] constitutive equations Z = ˜Z(C) were obtained for ferroelastic crystals in different cases. The entropy inequality (18) was analyzed by Liu’s theorem [27], and some constitutive relations were obtained, using Smith theorem [28], with the help of isotropic polynomial representations of proper constitutive functions satisfying the objectivity and material frame indifference principles (see [29]-[31]). In [10] the constitutive relation (12) for the total stress tensor was obtained expanding the free energy in Taylor series with respect to a particular natural state. In [12] the most general expression for G in the case of one-domain ferroelastic crystals (i.e., r = s = 1) was explicitly calculated (see equ.

(3.24)) in the following form: τ^{Γ}Γ˙ij = aδij+ btij + cΓij + N (q, ∇θ, t, Γ), where
τ^{Γ} denotes the relaxation time for the spontaneous strain field, the coefficients a, b, c
depend on the temperature θ and the set of invariants built on t, ∇θ, Γ, q (see (3.18),
(3.22) and (3.25)), while the non-linear part N depends also on t, ∇θ, Γ, q and can
be expanded into a polynomial expression with coefficients depending on θ and the same
invariants. The linearized theory (N = 0, a = 0) was considered explicitly in [13].

4. A geometric model for ferroelastic crystals

Now, we present a short review of a geometric model for ferroelastic crystals elaborated in [1], where following [2]-[4], introducing the concepts of process and transformation, we have derived the expressions for the existence of an entropy function and the entropy 1-form. We have considered a material point and we have defined the state space at time t as the set Btof all state variables which ”fit” the configuration of the element at time t. Bt

is assumed to have the structure of a finite dimensional manifold. The ”total state space”

is the disjoint union B =S

t{t} × Bt with a given natural structure of fibre bundle over R, where time flows [2]-[4]. If the instantaneous state space Btdoes not vary in time (i.e.

there is an abstract space B such that Bt' B for all instant of time t), then the total state space B has the topology of the Cartesian product B ' R × B (see [2]-[4]).

Moreover, we consider an abstract space of processes [2]-[6], i.e. a set Π of functions
P_{t}^{i} : [0, t] → G, where [0, t] is any time interval, the space G being a suitable target
space defined by the problem under consideration, i a label ranging in an unspecified
index set for all allowed processes and t ∈ R the so called duration of the process. Then,
a continuous function is defined (see [2]-[8])

(20) χ : (t, P_{t}^{i}) ∈ R × Π → ρ^{i}t∈ C^{0}(B, B),

with ρ^{i}_{t}: b ∈ D^{i}_{t}⊆ B → ρ^{i}_{t}(b) = b_{t}∈ R^{i}_{t}⊆ B, so that for any instant of time t and
for any process P_{t}^{i} ∈ Π a continuous mapping, ρ^{i}_{t}, called transformation induced by the
processis generated, which gives point by point a correspondence between the initial state
b and the final state ρ^{i}_{t}(b) = bt. Now, we introduce a function of time

(21) λ^{i}_{b}(τ ) =

b if τ = 0 with b ∈ Dt^{i}

ρ^{i}_{t}(b) if τ ∈]0, t]

such that the transformation for the medium is given by δ : R −→ R × B
(22) δ : τ ∈ R −→ δ(τ ) = (τ, λ^{i}b(τ )) ∈ R × B.

With these positions the transformation is interpreted as a curve δ in the union of all state spaces such that it intersects the instantaneous state space just once. In [1], taking into account the nonconventional thermodynamical model developed in section 3 of this paper,

it was assumed that the state variables are the deformation gradient F, the internal energy e (by a Legendre transformation the temperature θ was replaced with the internal energy e), the vector β = ∇θ, the heat flux vector q and the Anisotropy-Grain tensor Γ in the case that one type (size) of grain ( α = 1) and one kind of anisotropy (β = 1). Then, the full state space is

(23) B = Lin(V) ⊕ R ⊕ V ⊕ V ⊕ W,

where W is a vector space accounting for the internal variable Γ. In the general case
of α grains (α = 1, 2, ..., r) and β anisotropies (β = 1, 2, ..., s), W = ⊗_{α,β}T_{2}^{0}(V) is
given by r.s copies of T_{2}^{0}(V), V ' R^{3} , each one corresponding to a grain specie
α with anisotropy β, being T_{2}^{0}(V) a rank-2 tensor. Accordingly our state variables are
(F, e, ∇θ, q, Γ) and the process P_{t}^{i}is described by the following functions

P_{t}^{i}= [L(τ ), h(τ ), γ(τ ), Q(τ ), Λ(τ )], where h(τ ) = −∇ · q, γ(τ ) = ˙β.

The space G is given by G = Lin(V) ⊕ R ⊕ V ⊕ V ⊕ W. Moreover, the constitutive functions θ , t , Q and Λ are defined in the following way

θ : R × B −→ R^{++} t : R × B −→ Sym(V)
Q : R × B −→ V Λ : R × B −→ W,

where R^{++} is the set of real positive numbers, V and W are vector spaces accounting
for Q and Λ, respectively.

In this paper we assume that for each pair (P_{t}^{i}, b), the following dynamical system holds

(24)

F = L(τ )F(τ )˙

µ ˙e = t(δ) · L(τ ) + h(τ ) β = γ(τ )˙

q = Q(δ)˙ Γ = Λ(δ),˙

differing from that one presented in the previous paper [1], because in the rate equations of the system (24) for the heat flux and the anisotropy-grain field we have taken into con- sideration the material derivatives of these quantities and not the Zaremba-Jaumann time derivatives as in (17) (see [29]-[31] for this choice). Equation (24)2is given by (15), when the heat radiation per unit of mass is disregarded.

In this paper, as new results, we derive the linear morphism G, defined on the fibre bun-
dle of the process determined by the system (24), and the transformation induced by the
process ρ^{i}_{t}(b). The linear morphism G, defined in the following way

G : B × G ' T B −→ T B, has the following form

(25) G : (F, e, β, q, Γ, L, h, γ, Q, Λ) → (F, e, β, q, Γ, ˙F, ˙e, ˙β, ˙q, ˙Γ), which in matrix form is expressed by:

F, e, β, q, Γ, ˙F, ˙e, ˙β, ˙q, ˙ΓT

=

I 0

0 A

(F, e, β, q, Γ, L, h, γ, Q, Λ)^{T},

with

(26) A =

F 0 0 0 0

t µ

1

µ 0 0 0

0 0 1 0 0

0 0 0 1 0

0 0 0 0 1

.

The transformation ρ^{i}_{t}(b) is given by (see [4]):

(27) ρ^{i}_{t}(b) =

F = Rt

0[L(τ )F(τ )] dt e = Rt

0 1

µ[t(δ) · L(τ ) + h(τ )] dt β = Rt

0[γ(τ )] dt q = Rt

0[Q(δ)] dt Γ = Rt

0[Λ(δ)] dt.

In this geometrical structure, following standard procedures (see [2]-[4] and [8]), in [1] an

”entropy function” was introduced, related to a transformation between the initial state b
and the state ρ^{i}_{t}(b) = bt, by setting:

(28) s(ρ^{i}_{t}, b, t) = −
Z t

0

1

µ∇·Jsdτ = Z t

0

− 1

µθ∇·qdτ + Z t

0

1

µθ^{2}q·∇θdτ −
Z t

0

1 µ∇·kdτ, which in turn defines a 1-form Ω in R × B called the entropy 1-form. Using (24)2we have

−∇ · q = µ ˙e − t · ( ˙FF^{−1}). So that the final expression for s(ρ^{i}_{t}, b, t) is
(29) s(ρ^{i}t, b, t) =

Z

δ

Ω with Ω = 1 θ h

−1

µtF^{−T}· dF + de + 1
µ(1

θq · ∇θ − θ∇ · k) i

dτ,
where the algebraic rule t · ( ˙FF^{−1}) = (tF^{−T}) · ˙F has been used, with F^{−T} = (F^{−1})^{T}
(T being matrix transposition). Expressions of t, q and k were derived in [10] (see also
[9], [11]-[13] in which ferroelastic crystals were studied in different cases). Thus, the
entropy function is now calculated as an integral along a path into the space R × B of all
thermodynamic variables together with the independent time variable. In components the
entropy 1-form Ω becomes:

(30) Ω = ω_{µ}dq^{µ}+ ω_{0}dt = ω_{A}dq^{A}, (A = 1, 2, ..., 6),
where

q^{A}= (F, e, ∇θ, q, Γ, t)
and

ω_{A}=

− 1

µθtF^{−T},1

θ, 0, 0, 0, 1

µθ^{2}q · ∇θ −1
µ∇ · k

. Thus, by differentiation a 2-form is derived:

(31) dΩ = 1

2Aµλdq^{µ}∧ dq^{λ}+ Eλdt ∧ dq^{λ}, where Aµλ= ∂µωλ− ∂λωµ; and Eλ= ∂0ωλ− ∂λω0.
Applying the closure conditions for the 1-form, we obtain the following necessary con-
ditions for the existence of the entropy function during the process under consideration

(32) ∂F

1 θ

= −∂e

h _{1}
µθtF^{−T}i

, ∂e

1

µθ^{2}q · ∇θ −1
µ∇ · k

= ∂

∂t

1 θ

,

(33) ∂t

h _{1}
µθtF^{−T}i

= − ∂

∂F

1

µθ^{2}q · ∇θ − 1
µ∇ · k

,

∂ωA

∂q^{B} = 0, (A = 1, 2, 6, B = 3, 4, 5).

If the entropy 1-form in (29) is closed and its coefficients are regular (i.e. they have no singularities), this form is exact and the existence of an upper-potential S satisfying the relation S(σt) − S(σ0) ≥ s is ensured (see [8]). Starting from the entropy 1-form, it is possible to investigate and to introduce an extended thermodynamical phase space in a suitable way (see [32]).

5. Clausius-Duhem inequality analysis and heat equation

In this section, taking into account the model developed in [10] for ferroelastic media, we exploit the Clausius-Duhem inequality in the case that one type (size) of grain ( α = 1) and one kind of anisotropy (β = 1) is taken into consideration. Applying a Maugin technique [17] (see also Coleman-Noll procedure in [18]) we derive the entropy flux, the residual inequality and the laws of state, where in a relevant result the contributions in the total stress tensor expressed in terms of internal variables are rewritten in terms of the macroscopic variables represented by the Duhamel-Neumann tensor stress and the non- linear Eulerian strain tensor. Finally, the heat equation in the first and the second form is worked out following Maugin in [17].

We consider the entropy inequality µ ˙S + ∇ · Js≥ 0, with Js= ^{q}_{θ}+ k. Taking into
account the positivity of θ > 0 we have

(34) µθ ˙S + ∇ · (θJs) − Js· ∇θ ≥ 0.

Using in (34) the free energy expression Ψ = e − θS, the internal energy balance equation (15) and the entropy flux density, we obtain

(35) −µ( ˙Ψ + ˙θS) + p(i)+ ∇ · (θk) − Js· ∇θ ≥ 0.

Taking into account that Ψ is a constitutive function of (E, θ, ∇θ, q, Γ) we have

−µ_{∂Ψ}

∂E· ˙E +∂Ψ

∂θ

θ +˙ ∂Ψ

∂∇θ · ˙∇θ +∂Ψ

∂q · ˙q +∂Ψ

∂Γ· ˙Γ

− µ ˙θS+

(36) +(T − σ^{T E}− σ^{HA}) · ˙FF^{−1}+ ∇ · (θk) − Js· ∇θ ≥ 0.

Now, using the following expression for the time rate of nonlinear strain tensor (see [33]) (37) E = D −˙

EL + L^{T}E

= Sym( ˙FF^{−1}) − (E ˙FF^{−1}+ F^{−T}F˙^{T}E),

or in components E˙ij = Dij − (Eikvk,j+ Ejkvk,i), with D = ^{1}_{2} L +^{T} L , we
have

∂Ψ

∂E· ˙E = ∂Ψ

∂E· ˙FF^{−1}− E ˙FF^{−1}− F^{−T}F˙^{T}E

=

(38) =

_{∂Ψ}

∂EF^{−T}

−
E^{T}∂Ψ

∂EF^{−T}

−h E

_{∂Ψ}

∂E

T

F^{−T}
i^{}

· ˙F,

where E^{T} = E, ^{∂Ψ}_{∂E} =

∂Ψ

∂E

^{T}

and the matrix rule A · (BC) = B · (AC^{T}) = C · (B^{T}A) has been used.

Substituting equation (38) in (36) we obtain the final form for Clausius Duhem inequality:

−µ_{∂Ψ}

∂E− 2E∂Ψ

∂E

+

T − σ^{T E}− σ^{HA}i

F^{−T}· ˙F − µ ∂Ψ

∂θ + S

θ˙

(39) −µ ∂Ψ

∂∇θ · ∇ ˙θ − µ∂Ψ

∂q · ˙q − µ∂Ψ

∂Γ · ˙Γ + ∇ · (θk) − Js· ∇θ ≥ 0.

As T, σ^{T E}σ^{HA}, and S are assumed not to depend on F, ˙˙ θ, ∇ ˙θ, while the remaining
coefficients in (39) may in general depend on their respective factors and (39) has to remain
in one sign for any F, ˙˙ θ, ∇ ˙θ, taking into account equation (13), we obtain

(40) T = µ∂Ψ

∂E,

(41) σ^{T E}+ σ^{HA}= 2µE∂Ψ

∂E= 2ET,

(42) ∂Ψ

∂θ = −S, ∂Ψ

∂∇θ = 0.

Equations (40)-(42) are the laws of state. In (41) as new result the sum of σ^{T E}and σ^{HA}
expressed in terms of internal variables is derived in terms of the macroscopic variables
represented by the Duhamel-Neumann tensor stress T and the non-linear Eulerian strain
tensor E. At this point ”it is astute to select” the extra entropy flux density as (see [17])

(43) k = 0,

so that (39) reduces to the following residual dissipation inequality

(44) Φ = −µ∂Ψ

∂q · ˙q − µ∂Ψ

∂Γ· ˙Γ − Js· ∇θ ≥ 0.

These results are in agreement with the results obtained in [10] as a consequence of Liu’s
theorem. Very often Φ is split in two parts (”resulting thus in stronger conditions”)
(45) Φintr = −Π^{q}·q − η · ˙˙ Γ ≥ 0, Φth= −Js·∇θ ≥ 0, with Π^{q}= µ∂Ψ

∂q, and η = µ∂Ψ

∂Γ, where, in some sense, we recognize the different qualitative nature of the two classes of dissipative processes. Φintr and Φth are the intrinsic and thermal dissipations, respec- tively. Inequalities (45) govern dissipative processes and are in the standard bilinear form in terms of fluxes and associated forces: P

βXβYβ ≥ 0, as used in standard irreversible thermodynamics.

Now, in order to obtain the heat equation, we observe that it is none other than a form of energy balance equation. Indeed, on using the free energy expression Ψ = e − θS, its time derivative and the laws of state in the energy balance equation or, equivalently, ”just comparing” entropy inequality (34) and the residual dissipation inequality (44) we deduce the first general form of the heat equation

(46) µθ ˙S + ∇ · (θJs) = Φintr,

where ”the intrinsic dissipation acts like a body source of heat”. Now, using the state law (42)1and taking into account that the entropy S is a constitutive function of (F, θ, q, Γ), we have

(47) S = −˙

∂^{2}ψ

∂F∂θ· ˙F +∂^{2}ψ

∂θ^{2}θ +˙ ∂^{2}ψ

∂q∂θ· ˙q + ∂^{2}ψ

∂Γ∂θ· ˙Γ

.

Finally, substituting equation (47) in (46) and setting C = −µθ^{∂}_{∂θ}^{2}^{Ψ}_{2}, τ = µ_{∂θ∂E}^{∂}^{2}^{Ψ},
l = µ_{∂θ∂q}^{∂}^{2}^{Ψ}, m = µ_{∂θ∂Γ}^{∂}^{2}^{Ψ}, we obtain the second form of the heat equation in the following
compact form:

(48) C ˙θ + ∇ · (θJs) = Φte+ Φtq+ ΦtΓ, where
(49) Φte= θτ · ˙E, Φtq = (θl − Π^{q}) · ˙q, ΦtΓ= (θm − η) · ˙Γ.

Here the terms Φte, Φtqand ΦtΓrepresent the thermoelastic dissipation (due to the thermal and elastic phenomena), the dissipation due to the thermal phenomena and the dissipation due to the interaction between the thermal and the dislocation phenomena, respectively.

The non-negativity of the specific heat C follows from the concavity of Ψ with respect to
θ (^{∂}_{∂θ}^{2}^{ψ}2 ≤ 0).

References

[1] L. Restuccia, M. Francaviglia, ”Entropy function of heterogeneous and anisotropic nonlinear ferroelastic crystals”, in Series on advances in mathematics for applied sciences 69, edited by M. Primicerio, R. Spigler, V. Valente (World Scientific, New Jersey, London, Singapore, 2005).

[2] M. Dolfin, M. Francaviglia and P. Rogolino, ”A geometric perspective on irreversible thermodynamics with internal variables”, J. Non-Equilib. Thermodyn. 23, 250 (1998).

[3] M. Dolfin, M. Francaviglia and P. Rogolino, ”A geometric model on the thermodynamics of simple materi- als”, Periodica Polytechnica Series Mech. Eng. 43, 29 (1999).

[4] V. Ciancio, M. Dolfin, M. Francaviglia and P. Rogolino, ”Thermodynamic transformations in magnetically polarizable undeformable body”, J. Non-Equilib. Thermodyn., 26, 255 (2001).

[5] W. Noll, ”A mathematical theory of the mechanical behaviour of continuous media”, Arch. Rat. Mech. Anal., 2, 197 (1958).

[6] B. D. Coleman, M. E. Gurtin, ”Thermodynamics with internal state variables”, J. Chem. Phys., 47, 597 (1967).

[7] W. Noll, ”A new mathematical theory of simple materials”, Arch. Rat. Mech. Anal. 48, 1 (1972).

[8] B. D. Coleman, D. R. Owen, ”A mathematical foundation for thermodynamics”, Arch. Rat. Mech. Anal. 54, 1 (1974).

[9] B. Maruszewski, L. Restuccia, ”On a nonconventional model of ferroelastic crystals”, in Mechanika, 59, edited by A. Radowicz (Zeszyty Naukowe Politechniki Swietokrzyskiej, Kielce, Poland, 1995).

[10] L. Restuccia, B. Maruszewski, ”On a form of the stress tensor in a heterogeneous and anisotropic nonlinear thermoelastic solid”, Journal of Technical Physics 38 (4), 711 (1997).

[11] L. Restuccia, B. Maruszewski, ”Material thermodynamical description of ferroelastics”, in Mechanika, 66, edited by A. Radowicz (Zeszyty Naukowe Politechniki Swietokrzyskiej, Kielce, Poland, 1998).

[12] L. Restuccia, B. Maruszewski, ”Nonlinear thermoelasticity of ferroelastics”, Mechanics Research Commu- nications25 (2), 137 (1998).

[13] B. Maruszewski, L. Restuccia, ”Wave propagation in a ferroelastic body” in Proceedings of X INCOWAS- COM ’99, edited by V. Ciancio, A. Donato, F. Oliveri and S. Rionero (World Sientific, Singapore, New Jersey, London, Hong-Kong, 1999).

[14] B. Maruszewski, ”On an anysotropy-grain tensor”, Physics State Solid (b) 178, 265 (1993).

[15] M. Dolfin, M. Francaviglia and L. Restuccia, ”Thermodynamics of deformable dielectrics with a non- Euclidean structure as internal variable”, Technische Mechanik 24, 137 (2004).

[16] M. Francaviglia, L. Restuccia and P. Rogolino, ”Entropy production in polarizable bodies with internal variables”, Journal of Non-Equilibrium Thermodynamics 29, 221 (2004).

[17] G. A. Maugin, ”Internal variables and dissipative structures”, J. Non-Equilib. Thermodyn. 15 (2), 173 (1990).

[18] B. D. Coleman, W. Noll, ”The thermodynamics of elastic materials with heat conduction and viscosity”, Arch. Rat. Mech. Anal.13, 167 (1963).

[19] V. B. John, Introduction to engineering materials (MacMillan Co., New York, 1983) [20] L. Landau, E. Lifchitz, Physique statistique (Editions MIR, U.R.S.S., 1967).

[21] D. R. Askeland, The science and engineering of materials (PWS-Kent, Boston, 1984)

[22] C. Truesdell, W. Noll, The non-linear field theories of mechanics, Handbuch der Physik, III/3 (Springer, Berlin, Heidelberg, New York, 1965)

[23] W. Muschik, C. Papenfuss, H. Ehrentraut, Concepts of continuum thermodynamics (Kielce, Poland, 1996).

[24] W. Muschik, Aspects of non-equilibrium thermodynamics (World Scientific, Singapore, 1990).

[25] W. Muschik, “Fundamentals of non-equilibrium thermodynamics,” in Non-equilibrium thermodynamics with applications to solidsedited by W. Muschik, CISM Courses and Lectures 336 (Springer Verlag, Wien - New York, 1993).

[26] W. Muschik, C. Papenfuss, H. Ehrentraut, ”‘A sketch of continuum thermodynamics”’, J. Non-Newtonian fluid Mech., 96, 255 (2001).

[27] I-Shih Liu, ” The method of Lagrange multipliers for exploitation of the entropy principle”, Arch. Rat. Mech.

Anal.46, 131 (1972).

[28] G. F. Smith, ”On isotropic functions of symmetric tensors, skew-symmetric tensors and vectors”, Int. J.

Engng. Sci.9, 899 (1971).

[29] W. Muschik, L. Restuccia, ”Changing the observer and moving materials in continuum physics: objectivity and frame indifference”, Technische Mechanik 22, 152 (2002).

[30] H. Herrmann, W. Muschik, G. R¨uckner, L. Restuccia, ”Constitutive mappings and the non-objective part of material frame indifference” in Trends in Continuum Physics’04 (TRECOP’04) edited by B. T.

Maruszewski, W. Muschik, A. Radowicz (WNPP, Poznan, Poland, 2004)

[31] W.Muschik, L. Restuccia, ”Systematic Remarks on Objectivity and Frame-Indifference. Liquid Crystal The- ory as an Example”, Archive of Applied Mechanics, 2007.

[32] S. Preston, J.Vargo, ”Indefinite metric of R. Mrugala and the geometry of thermodynamical phase state”, in Proc.s of International Conference and Summerschool Thermal Theories of Continua: Survey and Devel- opments’05 (THERMOCON ’05), edited by V. Ciancio, M. Francaviglia, W. Muschik and L. Restuccia ( Supplemento Atti Accademia Peloritana dei Pericolanti di Messina, 2007).

[33] G.A. Maugin, Continuum mechanics of electromagnetic solids, North-Holland Series in Applied Mathemat- ics and Mechanics (Amsterdam, 1988).

[a] Mauro Francaviglia

Universit`a degli Studi di Torino Dipartimento di Matematica Via Carlo Alberto 10 10123 Torino, Italy

[b] Liliana Restuccia

Universit`a degli Studi di Messina Dipartimento di Matematica Salita Sperone 31

98166 Messina, Italy

* E-mail: lrest@dipmat.unime.it Presented: September 29, 2005 Published on line: February 01, 2008